#------------------------------------------------------------------------------
#$Date: 2016-03-26 20:56:05 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180456 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/25/7212547.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7212547
loop_
_publ_author_name
'Galloway, Kyle W.'
'Moggach, Stephen A.'
'Parois, Pascal'
'Lennie, Alistair R.'
'Warren, John E.'
'Brechin, Euan K.'
'Peacock, Robert D.'
'Valiente, Rafael'
'González, Jesús'
'Rodríguez, Fernando'
'Parsons, Simon'
'Murrie, Mark'
_publ_section_title
;
 Pressure-induced switching in a copper(ii) citrate dimer
;
_journal_issue                   9
_journal_name_full               CrystEngComm
_journal_page_first              2516
_journal_paper_doi               10.1039/c001376e
_journal_volume                  12
_journal_year                    2010
_chemical_formula_moiety         'C12 H8 Cu2 O14, 4(C H6 N3), 2(H2 O)'
_chemical_formula_sum            'C16 H36 Cu2 N12 O16'
_chemical_formula_weight         779.63
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_audit_creation_date             08-04-02
_audit_creation_method           CRYSTALS_ver_12.85
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.5200(4)
_cell_length_b                   14.4315(7)
_cell_length_c                   18.012(3)
_cell_measurement_reflns_used    5214
_cell_measurement_temperature    293
_cell_measurement_theta_max      17
_cell_measurement_theta_min      2
_cell_volume                     2994.5(5)
_computing_cell_refinement       'SAINT (Siemens ,1995)'
_computing_data_collection       'SMART (Siemens, 1993)'
_computing_data_reduction        'SAINT (Siemens ,1995)'
_computing_molecular_graphics    'CAMERON (Watkin et al., 1996)'
_computing_publication_material  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_refinement  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_solution    'Refined from ambient pressure coordinates'
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.581
_diffrn_measured_fraction_theta_max 0.545
_diffrn_measurement_device       'Bruker SMART'
_diffrn_measurement_device_type  Area
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           ' synchrotron '
_diffrn_radiation_wavelength     0.47540
_diffrn_reflns_av_R_equivalents  0.081
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            19261
_diffrn_reflns_theta_full        13.327
_diffrn_reflns_theta_max         17.307
_diffrn_reflns_theta_min         2.034
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    1.512
_exptl_absorpt_correction_T_max  0.86
_exptl_absorpt_correction_T_min  0.60
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Siemens, 1996)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    1.729
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1608
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.32
_refine_diff_density_min         -0.34
_refine_ls_extinction_method     None
_refine_ls_goodness_of_fit_ref   0.9194
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     214
_refine_ls_number_reflns         1667
_refine_ls_number_restraints     152
_refine_ls_R_factor_all          0.0576
_refine_ls_R_factor_gt           0.0389
_refine_ls_shift/su_max          0.000717
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
Method= Modified Sheldrick
w=1/[σ²(F²) + ( 0.04P)² + 8.03P]
,where P=(max(Fo²,0) + 2Fc²)/3
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1091
_refine_ls_wR_factor_gt          0.0944
_refine_ls_wR_factor_ref         0.1091
_reflns_limit_h_max              14
_reflns_limit_h_min              0
_reflns_limit_k_max              18
_reflns_limit_k_min              0
_reflns_limit_l_max              12
_reflns_limit_l_min              0
_reflns_number_gt                1277
_reflns_number_total             1677
_reflns_threshold_expression     I>2.0σ(I)
_oxford_diffrn_Wilson_B_factor   1.79
_oxford_diffrn_Wilson_scale      39.85
_oxford_refine_ls_r_factor_ref   0.0576
_oxford_refine_ls_scale          0.5379(17)
_oxford_reflns_number_all        1667
_oxford_reflns_threshold_expression_ref I>-10.0\s(I)
_oxford_structure_analysis_title 'pcu201 in Pbca'
_cod_data_source_file            c001376e.txt
_cod_data_source_block           pcu201
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      'P b c a '
_cod_database_code               7212547
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-x,-y,-z
-x+1/2,y+1/2,z
x+1/2,-y+1/2,-z
x,-y+1/2,z+1/2
-x,y+1/2,-z+1/2
-x+1/2,-y,z+1/2
x+1/2,y,-z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
Cu1 Cu 0.50597(3) 0.52337(3) 0.57658(6) 0.0299 1.0000 Uani . .
C1 C 0.7107(2) 0.5354(2) 0.4873(3) 0.0299 1.0000 Uani D U
C2 C 0.7877(3) 0.5326(3) 0.5569(3) 0.0354 1.0000 Uani D U
C3 C 0.7344(3) 0.5692(3) 0.6286(3) 0.0384 1.0000 Uani D U
C4 C 0.7733(3) 0.4984(3) 0.4191(3) 0.0308 1.0000 Uani D U
C5 C 0.7102(3) 0.5192(3) 0.3474(3) 0.0323 1.0000 Uani D U
C6 C 0.6762(3) 0.6376(2) 0.4755(4) 0.0303 1.0000 Uani D U
C7 C 0.5525(3) 0.8490(3) 0.6653(3) 0.0359 1.0000 Uani D U
C8 C 0.4234(3) 0.1793(3) 0.6811(3) 0.0370 1.0000 Uani D U
N1 N 0.4990(3) 0.8132(3) 0.6062(4) 0.0558 1.0000 Uani D U
N2 N 0.6664(3) 0.8388(3) 0.6733(4) 0.0437 1.0000 Uani D U
N3 N 0.4947(3) 0.8959(3) 0.7162(4) 0.0560 1.0000 Uani D U
N4 N 0.3101(3) 0.1946(2) 0.6889(4) 0.0383 1.0000 Uani D U
N5 N 0.4796(3) 0.2106(3) 0.6233(4) 0.0458 1.0000 Uani D U
N6 N 0.4785(3) 0.1312(3) 0.7317(4) 0.0532 1.0000 Uani D U
O1 O 0.6295(2) 0.5470(2) 0.6445(3) 0.0412 1.0000 Uani D U
O2 O 0.7931(2) 0.6179(2) 0.6699(3) 0.0428 1.0000 Uani D U
O3 O 0.6011(2) 0.4984(2) 0.3426(3) 0.0417 1.0000 Uani D U
O4 O 0.7608(2) 0.5559(3) 0.2957(3) 0.0432 1.0000 Uani D U
O5 O 0.5837(2) 0.66457(17) 0.5056(3) 0.0328 1.0000 Uani D U
O6 O 0.7462(2) 0.68791(18) 0.4402(3) 0.0378 1.0000 Uani D U
O7 O 0.61036(18) 0.48020(15) 0.4996(3) 0.0360 1.0000 Uani D U
O8 O 0.6818(3) 0.1967(2) 0.0526(4) 0.0515 1.0000 Uani D .
H81 H 0.656(4) 0.1457(17) 0.041(3) 0.0500 1.0000 Uiso D .
H82 H 0.707(5) 0.218(3) 0.0136(16) 0.0500 1.0000 Uiso D .
H41 H 0.8490 0.5260 0.4169 0.0369 1.0000 Uiso . .
H42 H 0.7809 0.4324 0.4240 0.0369 1.0000 Uiso . .
H21 H 0.8558 0.5687 0.5467 0.0425 1.0000 Uiso . .
H22 H 0.8094 0.4692 0.5652 0.0425 1.0000 Uiso . .
H11 H 0.4253 0.8198 0.6010 0.0670 1.0000 Uiso . .
H12 H 0.5383 0.7834 0.5733 0.0670 1.0000 Uiso . .
H23 H 0.7010 0.8619 0.7114 0.0524 1.0000 Uiso . .
H24 H 0.7057 0.8091 0.6404 0.0524 1.0000 Uiso . .
H31 H 0.5306 0.9185 0.7539 0.0671 1.0000 Uiso . .
H32 H 0.4210 0.9038 0.7116 0.0671 1.0000 Uiso . .
H51 H 0.5526 0.1997 0.6185 0.0550 1.0000 Uiso . .
H52 H 0.4436 0.2422 0.5900 0.0550 1.0000 Uiso . .
H61 H 0.4417 0.1105 0.7698 0.0641 1.0000 Uiso . .
H62 H 0.5515 0.1203 0.7269 0.0641 1.0000 Uiso . .
H43 H 0.2740 0.1736 0.7272 0.0462 1.0000 Uiso . .
H44 H 0.2730 0.2254 0.6556 0.0462 1.0000 Uiso . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
C 0.0000 0.0010 2.3100 20.8439 1.0200 10.2075 1.5886 0.5687 0.8650 51.6512
0.2156 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
H 0.0000 0.0000 0.4930 10.5109 0.3229 26.1257 0.1402 3.1424 0.0408 57.7998
0.0030 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
N 0.0010 0.0010 12.2126 0.0057 3.1322 9.8933 2.0125 28.9975 1.1663 0.5826
-11.5290 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
O 0.0030 0.0020 3.0485 13.2771 2.2868 5.7011 1.5463 0.3239 0.8670 32.9089
0.2508 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
Cu 0.2890 0.6120 13.3380 3.5828 7.1676 0.2470 5.6158 11.3966 1.6735 64.8126
1.1910 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_site_symmetry_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O3 2_666 Cu1 O7 2_666 95.05(16) yes
O3 2_666 Cu1 O1 . 91.3(2) yes
O7 2_666 Cu1 O1 . 169.97(15) yes
O3 2_666 Cu1 O5 . 136.58(13) yes
O7 2_666 Cu1 O5 . 84.79(13) yes
O1 . Cu1 O5 . 85.26(16) yes
O3 2_666 Cu1 O7 . 151.91(13) yes
O7 2_666 Cu1 O7 . 85.02(10) yes
O1 . Cu1 O7 . 93.08(16) yes
O5 . Cu1 O7 . 71.48(11) yes
C2 . C1 C4 . 112.0(3) yes
C2 . C1 C6 . 106.7(3) yes
C4 . C1 C6 . 110.3(4) yes
C2 . C1 O7 . 109.2(4) yes
C4 . C1 O7 . 108.3(3) yes
C6 . C1 O7 . 110.4(2) yes
C1 . C2 C3 . 116.7(3) yes
C1 . C2 H21 . 107.6 no
C3 . C2 H21 . 107.6 no
C1 . C2 H22 . 107.6 no
C3 . C2 H22 . 107.6 no
H21 . C2 H22 . 109.5 no
C2 . C3 O1 . 118.8(4) yes
C2 . C3 O2 . 119.3(3) yes
O1 . C3 O2 . 121.9(4) yes
C1 . C4 C5 . 113.0(3) yes
C1 . C4 H41 . 108.6 no
C5 . C4 H41 . 108.6 no
C1 . C4 H42 . 108.6 no
C5 . C4 H42 . 108.6 no
H41 . C4 H42 . 109.5 no
C4 . C5 O3 . 118.5(4) yes
C4 . C5 O4 . 120.6(3) yes
O3 . C5 O4 . 120.9(5) yes
C1 . C6 O5 . 117.0(3) yes
C1 . C6 O6 . 117.2(3) yes
O5 . C6 O6 . 125.6(3) yes
N1 . C7 N2 . 119.9(4) yes
N1 . C7 N3 . 121.3(4) yes
N2 . C7 N3 . 118.7(4) yes
N4 . C8 N5 . 120.8(4) yes
N4 . C8 N6 . 119.3(4) yes
N5 . C8 N6 . 119.8(4) yes
C7 . N1 H11 . 120.0 no
C7 . N1 H12 . 120.0 no
H11 . N1 H12 . 120.0 no
C7 . N2 H23 . 120.0 no
C7 . N2 H24 . 120.1 no
H23 . N2 H24 . 119.9 no
C7 . N3 H31 . 120.0 no
C7 . N3 H32 . 119.9 no
H31 . N3 H32 . 120.1 no
C8 . N4 H43 . 120.0 no
C8 . N4 H44 . 120.0 no
H43 . N4 H44 . 120.0 no
C8 . N5 H51 . 120.0 no
C8 . N5 H52 . 120.0 no
H51 . N5 H52 . 120.0 no
C8 . N6 H61 . 120.0 no
C8 . N6 H62 . 120.0 no
H61 . N6 H62 . 120.0 no
C3 . O1 Cu1 . 127.2(4) yes
C5 . O3 Cu1 2_666 127.4(4) yes
Cu1 . O5 C6 . 105.4(2) yes
C1 . O7 Cu1 . 115.8(3) yes
C1 . O7 Cu1 2_666 118.2(3) yes
Cu1 . O7 Cu1 2_666 94.98(10) yes
H81 . O8 H82 . 104.6(10) no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Cu1 O3 2_666 1.934(5) yes
Cu1 O7 2_666 1.918(4) yes
Cu1 O1 . 1.907(4) yes
Cu1 O5 . 2.567(3) yes
Cu1 O7 . 1.939(4) yes
C1 C2 . 1.536(6) yes
C1 C4 . 1.522(6) yes
C1 C6 . 1.542(4) yes
C1 O7 . 1.421(3) yes
C2 C3 . 1.525(6) yes
C2 H21 . 0.960 no
C2 H22 . 0.960 no
C3 O1 . 1.283(4) yes
C3 O2 . 1.227(5) yes
C4 C5 . 1.513(6) yes
C4 H41 . 0.960 no
C4 H42 . 0.960 no
C5 O3 . 1.295(4) yes
C5 O4 . 1.219(6) yes
C6 O5 . 1.258(4) yes
C6 O6 . 1.257(5) yes
C7 N1 . 1.334(7) yes
C7 N2 . 1.329(4) yes
C7 N3 . 1.319(6) yes
C8 N4 . 1.331(4) yes
C8 N5 . 1.307(7) yes
C8 N6 . 1.310(6) yes
N1 H11 . 0.860 no
N1 H12 . 0.860 no
N2 H23 . 0.861 no
N2 H24 . 0.860 no
N3 H31 . 0.859 no
N3 H32 . 0.860 no
N4 H43 . 0.860 no
N4 H44 . 0.860 no
N5 H51 . 0.860 no
N5 H52 . 0.860 no
N6 H61 . 0.860 no
N6 H62 . 0.860 no
O8 H81 . 0.819(9) no
O8 H82 . 0.822(10) no
